Smart Materials, Adaptive Structures, and Intelligent Mechanical Systems


 Roxanne Scott
 1 years ago
 Views:
Transcription
1 Smart Materials, Adaptive Structures, and Intelligent Mechanical Systems Bishakh Bhattacharya & Nachiketa Tiwari Indian Institute of Technology Kanpur
2 Lecture 19 Analysis of an Orthotropic Ply
3 References for this Lecture 1. Analysis and Performance of Fiber Composites, Agarwal, B.D. and Broutman, L. J., John Wiley & Sons. 2. Mechanics of Composite Materials, Jones, R. M., Mc Graw Hill 3. Structural Analysis of Laminated Composites, Whitney, J. M., Technomic 4. Nonlinear Analyis of Plates, Chia, C., McGraw Hill International Book Company
4 Lecture Overview Transformation of stresses and strains Stress strain relations for a lamina with any orientation i Strength of an orthotropic lamina
5 Introduction Earlier, while discussing ssing the stress state in 2 D orthotropic materials, it was assumed that reference axes for measuring stresses and strains were coincident with material axes. In reality, that may not be the case. Hence, there is a need to develop stress strain relations in a 2 D orthotropic lamina oriented arbitrarily. Towards this goal, as a first step, we have to transform stresses and strains from material axes to arbitrary axes, and vice versa. Consider a tetrahedron with vertices ABCP. Its face ABC, with surface area A and, normal n (with direction cosines, n x x, n y y, and n z z), experiences is subjected to stress vector T, such that the total external force on face ABC is T A. Further, the x, y, and z components of T are T x, T y, and T z, respectively. Further, we assume that the length of normal to face ABC passing through P is h. Such a tetrahedron is shown in Figure 19.1.
6 Engineering Constants for a 2D Lamina B y T y n T x T x σ z σ x P A x C σ y z Fig. 19.1: Tetrahedron at Point P
7 Engineering Constants for a 2 D Orthotropic Lamina Further, we assume that the body is in equilibrium, and thus, other three faces experience normal and shear stresses. Given that the body is in equilibrium, we can write the following three equilibrium equations. σ xx An x + τ yx An y + τ zx An z = T x A τ xy An x + σ yy An y + τ zy An z = T y A τ xz An x + τ yz An y + σ zz An z = T z A, Eliminating A from above equations, we get Cauchy stress formulae, as follows. σ xx n x + τ yx n y + τ zx n z =Tn x =T x τ xy n x + σ yy n y + τ zy n z = Tn y =T y (Eq. 19.1) τ xz n x + τ yz n y + σ zz n z = Tn z =T z In Eq. 19.1, T x, T y, and T z, are x, y, and z, components of stress vector T. Further, T, can also be resolved in terms of its normal and tangential component, with respect to surface A. The normal component can be expressed as: σ n = T x n x + T y n y + T z n z (Eq. 19.2)
8 Engineering Constants for a 2 D Orthotropic Lamina Combining Equations 19.1 and 19.2, we can write the relation for normal stress as: σ n = σ xxn x2 + σ yyn y2 + σ zzn z2 + 2τ xyn xn y + 2τ yzn yn z + 2τ zxn zn x (Eq. (q 19.3) Eq can be used to transform normal stress from one set of axes to another set of axes. Now, let us consider Fig Here, we assume that the stress state at a point with respect to an arbitrary set of axes, x, y, and z is known. We would like to use this information to calculate the stress state with respect to natural material axes of the system. T y θ L x Fig. 19.2: Orientation of Natural Material Axes with reference to ArbitraryAxesAxes z, T
9 Engineering Constants for a 2 D Orthotropic Lamina From Fig. 19.2, it is seen that the material axis system is essentially a rotation of x y axes, around z axis by an angle θ. Thus the direction cosines for the material axis system (L T T ), T T with respect to x y z system are, cos θ,sin θ and 1. Thus, normal stresses σ xx, and σ yy can be written as: σ L = σ xx cos 2 θ + σ yy sin 2 θ +2τ xy cos θ sin θ (Eq. 19.4a) σ 2 2 T = σ xx sin θ + σ yy cos θ + 2τ xy cos θ sin θ (Eq. 19.4b) Using similar approach, we can also write the equation for shear stress can be written as as: τ LT = σ xx cos θ sin θ + σ yy cos θ sin θ + τ xy cos 2 θ sin 2 θ (Eq. 19.4c) Eqs. 19.4a c, can also be written in matrix form as: Eq. (19.5)
10 Engineering Constants for a 2 D Orthotropic Lamina Similar equations can also be used to transform strains from one coordinate system to another one. The strain transformation equations are: Eq. (19.6) In Equations 19.5 and 19.6, [M] is transformation matrix, and is defined as: Eq. (19.7) It may be noted here, that unlike stress transformation equations, strain transformation equations have a factor of ½ within strain vectors. This is because such a transformation requires usage of tensor strains, and not engineering strains. While mathematical definitions of normal tensor strain and normal engineering strains are identical, tensor shear strain is one half times that of engineering shear strain.
11 Transformation of Engineering Constants Now, that we have relations which can be used to transform strains from one system to other, we proceed to develop relations which will help us transform engineering constants. Pre multiplying Eq by [T] 1 on either sides, we get: [T] 1 {σ} L T = [T] 1 [T] {σ} x y or {σ} x y = [T] 1 {σ} L T (Eq. 19.8) where, {σ} L T and {σ} x y are stresses measured in x y, and L T reference frames, respectively. Further, as shown in earlier lecture, we can write stress strain relation as: {σ} L T = [Q] {ε} L T (Eq. 19.9) 9) Putting RHS of Eq in RHS of Eq. 19.8, we get: {σ} x y = [T] 1 [Q] {ε} L T (Eq )
12 Transformation of Engineering Constants And finally expressing {ε} L T in terms of {σ} x y, using appropriate transformations, in Eq , we get: {σ} x y = [T] 1 [Q] [T]{ε} x y or, {σ} x y = [Q]{ε} x y (Eq ) Equation helps us compute stresses measured in x y coordinate system in terms of strains measure in the same system. Here, [Q] is the transformed stiffness matrix, and its individual components are: Q 11 = Q 11 cos 4 θ + Q 22 sin 4 θ + 2(Q 12 +2Q 66 ) sin 2 θ cos 2 θ Q 22 = Q 11 sin 4 θ + Q 22 cos 4 θ + 2(Q 12 +2Q 66 ) sin 2 θ cos 2 θ Q 12 = (Q 11 + Q 22 4Q 66 )sin 2 θ cos 2 θ + Q 12 (cos 4 θ + sin 4 θ) Q = (Q 11 Q 22 2Q 12 2Q 66 )sin θ cos θ Q 66 (cos θ sin θ) Q 16 = (Q 11 Q 22 2Q 66 )sinθ cos 3 θ (Q 22 Q 12 2Q 66 )sin 3 θ cos θ Q 26 = (Q 11 Q 22 2Q 66 )sin 3 θ cos θ (Q 22 Q 12 2Q 66 )sin θ cos 3 θ (Eq ) 12)
13 Transformation of Engineering Constants Following observations can be made from Eq Unlike, [Q] matrix, [Q] matrix is fully populated. Terms Q 16, and Q 26 are identically zero. However, terms Q 16, and Q 26, are not necessarily zero, and their definition involves linear combinations of four elements of [Q] matrix. For a specially orthotropic lamina, i.e. when its loading direction coincides with lamina s material axes, application of normal stresses produce only normal strains, and application of shear stresses produce pure shear strains. For a generally orthotropic lamina, i.e. when loading direction and material axes are not coincidental, application of normal stresses produce normal as well as shear strains. This occurs because of non zero values for terms Q 16, and Q 26, which couple normal and shear responses. These terms are also known as cross coupling stiffness coefficients.
14 Transformation of Engineering Constants Using a transformation procedure similar to the one used to transform stiffness matrix [Q], we can also transform the compliance matrix [S] to an arbitrary coordinate system. The elements of transformed compliance matrix [S] are defined below. S 11 = S 11 cos 4 θ + S 22 sin 4 θ + (2S 12 + S 66 ) sin 2 θ cos 2 θ S 22 = S 11 sin 4 θ + S 22 cos 4 θ + (2S 12 + S 66 ) sin 2 θ cos 2 θ S 12 = (S 11 + S 22 S 66 )sin 2 θ cos 2 θ + S 12 (cos 4 θ + sin 4 θ) S = 2(2S S 22 4S 12 S 66 )sin θ cos θ + S 66 (cos θ + sin θ) S 16 = 2(2S 11 2S 22 S 66 )sinθ cos 3 θ 2(2S 22 2S 12 S 66 )sin 3 θ cos θ S 26 = 2(2S 11 2S 22 S 66 )sin 3 θ cos θ 2(2S 22 2S 12 S 66 )sin θ cos 3 θ (Eq )
15 Strength of an Orthotropic Lamina In isotropic materials, failure prediction requires calculating principal stresses or strains and comparing them to their respective allowable stress and strain limits. i In non isotropic materials such an approach does not work. The notion of principal stress makes no sense for these materials, as material strength changes withdirection direction, anddirection direction ofprincipal stress may not in most of the cases coincide with direction of maximum strength. For an isotropic material, we can fully describe allowable stress field by knowing the material s tensile, compressive and shear strength.
16 Failure in Isotropic v/s Transversely Isotropic Materials Similarly, for 2 D orthotropic materials, we evaluate allowable stress field in context of five different strengths of material measured with respect to its principal material directions. These are: Longitudinal tensile strength (σ LU ) Lateral or transverse tensile strength (σ TU ) Longitudinal compressive strength (σ LU ) Lateral or transverse compressive strength (σ LU ) In plane planeshear strength (τ LTU ) These material strength parameters for an orthotropic lamina These material strength parameters for an orthotropic lamina are its fundamental material properties.
17 Failure in Orthotropic Materials Similar to isotropic materials, several theories have been developed to predict pedctfailure auein orthotropic ot op materials. a Some of the more oewidely used theories are based on maximum stress, maximum strain, and maximum work. Maximum Stress Theory: As per this theory, failure will occur once stresses measured with respect to principal material axes, exceed their respective allowable limits. Thus, for failure at least one of the following conditions must be violated. For tensile loads: σ L < σ LU, σ T < σ TU, τ LT < τ LTU. For compressive loads: σ L < σ LU, σ T < σ TU. (Eq ) One limitation of this theory is that different modes of potential failure do not interact with each other.
18 Failure in Orthotropic Materials Maximum m Strain Theory: Asperthis theory, failure will occur roncestrains measured with respect to principal material axes, exceed their respective allowable limits. Thus, for failure, at least one of the following five conditions must be violated. For normal tensile strains the conditions are: ε L < ε LU, ε T < ε TU, γ LT < γ LTU. And if normal strains are compressive, then failure criteria are: ε L < ε LU, ε T < ε TU. (Eq ) If material is linearly elastic, then Eq can be re written as: ε L < σ LU /E L, ε T < σ TU /E T, γ LT < τ LTU /G LT. ε L < σ LU /E L, ε T < σ TU /E T. (Eq ) Predictions from maximum stress and maximum strain theories are very similar, with minor differences being attributable to role of Poisson s ratio. This is true for linear elastic materials. For non linear elastic materials, Eq should not be used, and significant difference should be expected between results from these two theories.
19 Failure in Orthotropic Materials Tsai Hill or Maximum m Work Theory: As per this theory, failure occurs when the following inequality condition is violated. (σ L /σ LU ) 2 (σ L /σ LU ) (σ T /σ TU ) + (σ T /σ TU ) 2 + (τ LT /τ LTU ) 2 < 1 (Eq ) Here, if normalstresses arecompressive then compressive strength should be used in the equation. Also, if the lamina is subjected to unidirectional normal stress, then above equation can be simplified as: (cos 2 θ/σ LU ) 2 (cosθ sinθ/σ LU ) 2 + (sin 2 θ /σ TU ) 2 + (cosθ sinθ/τ LTU ) 2 < (1/ σ x ) 2 (Eq ) Unlike maximum stress and strain theories, Eq provides a single criterion for predicting failure. It also accounts for interaction between differentstrengths ofthematerial material. Predictions ofstrength fromthis theoryare slightly lesser than those from maximum stress and maximum strain theories. All the theories discussed till so far work only for a lamina subjected to bi axial stress state and not for tri axial stress state.
20 What you learnt in this lecture? Transformation of stress and strains Stress strain relations for a lamina with any orientation i Strength of an orthotropic lamina
Composite Structures. Indian Institute of Technology Kanpur
Mechanics of Laminated Composite Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 23 Analysis of an Orthotropic Ply Lecture Overview Introduction Engineering constants for an 2
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 15 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 34 Thermal Stresses in Plates Lecture Overview Introduction Mechanical and Thermal Strains
More informationSmart Materials, Adaptive Structures, and Intelligent Mechanical Systems
Smart Materials, Adaptive Structures, and Intelligent Mechanical Systems Bishakh Bhattacharya & Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 32 Energy Methods References for this Lecture
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 36 Hygrothermal Stresses in Plates Lecture Overview Introduction Hygrothermal Strains Stiffness
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationUnit IV State of stress in Three Dimensions
Unit IV State of stress in Three Dimensions State of stress in Three Dimensions References Punmia B.C.,"Theory of Structures" (SMTS) Vol II, Laxmi Publishing Pvt Ltd, New Delhi 2004. Rattan.S.S., "Strength
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationStress, Strain, Mohr s Circle
Stress, Strain, Mohr s Circle The fundamental quantities in solid mechanics are stresses and strains. In accordance with the continuum mechanics assumption, the molecular structure of materials is neglected
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationComposite Structures. Indian Institute of Technology Kanpur
Mechanics of Laminated Composite Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 21 Behavior of Ribbon Fiber Composites Ribbon Reinforced Composites: Introduction Quite often,
More informationLecture 8. Stress Strain in Multidimension
Lecture 8. Stress Strain in Multidimension Module. General Field Equations General Field Equations [] Equilibrium Equations in Elastic bodies xx x y z yx zx f x 0, etc [2] Kinematics xx u x x,etc. [3]
More information9 Strength Theories of Lamina
9 trength Theories of Lamina 9 TRENGTH O ORTHOTROPIC LAMINA or isotropic materials the simplest method to predict failure is to compare the applied stresses to the strengths or some other allowable stresses.
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationME 7502 Lecture 2 Effective Properties of Particulate and Unidirectional Composites
ME 75 Lecture Effective Properties of Particulate and Unidirectional Composites Concepts from Elasticit Theor Statistical Homogeneit, Representative Volume Element, Composite Material Effective Stress
More informationPrincipal Stresses, Yielding Criteria, wall structures
Principal Stresses, Yielding Criteria, St i thi Stresses in thin wall structures Introduction The most general state of stress at a point may be represented by 6 components, x, y, z τ xy, τ yz, τ zx normal
More informationBasic Equations of Elasticity
A Basic Equations of Elasticity A.1 STRESS The state of stress at any point in a loaded bo is defined completely in terms of the nine components of stress: σ xx,σ yy,σ zz,σ xy,σ yx,σ yz,σ zy,σ zx,andσ
More information3D and Planar Constitutive Relations
3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace
More information3D Elasticity Theory
3D lasticity Theory Many structural analysis problems are analysed using the theory of elasticity in which Hooke s law is used to enforce proportionality between stress and strain at any deformation level.
More informationHygrothermal stresses in laminates
Hygrothermal stresses in laminates Changing environment conditions (temperature and moisture) have an important effect on the properties which are matrix dominated. Change in temperaturet and moisture
More informationUNIVERSITY OF SASKATCHEWAN ME MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich
UNIVERSITY OF SASKATCHEWAN ME 313.3 MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich A CLOSED BOOK EXAMINATION TIME: 3 HOURS For Marker s Use Only LAST NAME (printed): FIRST
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationARC 341 Structural Analysis II. Lecture 10: MM1.3 MM1.13
ARC241 Structural Analysis I Lecture 10: MM1.3 MM1.13 MM1.4) Analysis and Design MM1.5) Axial Loading; Normal Stress MM1.6) Shearing Stress MM1.7) Bearing Stress in Connections MM1.9) Method of Problem
More informationMechanics of Earthquakes and Faulting
Mechanics of Earthquakes and Faulting www.geosc.psu.edu/courses/geosc508 Surface and body forces Tensors, Mohr circles. Theoretical strength of materials Defects Stress concentrations Griffith failure
More informationComposites Design and Analysis. Stress Strain Relationship
Composites Design and Analysis Stress Strain Relationship Composite design and analysis Laminate Theory Manufacturing Methods Materials Composite Materials Design / Analysis Engineer Design Guidelines
More informationMechanical Behavior of Composite Tapered Lamina
International Journal of Engineering Research and Development eissn: 2278067X, pissn: 2278800X, www.ijerd.com Volume 10, Issue 8 (August 2014), PP.1927 Mechanical Behavior of Composite Tapered Lamina
More informationStress/Strain. Outline. Lecture 1. Stress. Strain. Plane Stress and Plane Strain. Materials. ME EN 372 Andrew Ning
Stress/Strain Lecture 1 ME EN 372 Andrew Ning aning@byu.edu Outline Stress Strain Plane Stress and Plane Strain Materials otes and News [I had leftover time and so was also able to go through Section 3.1
More informationFinite Element Method in Geotechnical Engineering
Finite Element Method in Geotechnical Engineering Short Course on + Dynamics Boulder, Colorado January 58, 2004 Stein Sture Professor of Civil Engineering University of Colorado at Boulder Contents Steps
More informationStress, Strain Stress strain relationships for different types of materials Stress strain relationships for a unidirectional/bidirectional lamina
Chapter 2 Macromechanical Analysis of a Lamina Stress, Strain Stress strain relationships for different types of materials Stress strain relationships for a unidirectional/bidirectional lamina Islamic
More information16.20 HANDOUT #2 Fall, 2002 Review of General Elasticity
6.20 HANDOUT #2 Fall, 2002 Review of General Elasticity NOTATION REVIEW (e.g., for strain) Engineering Contracted Engineering Tensor Tensor ε x = ε = ε xx = ε ε y = ε 2 = ε yy = ε 22 ε z = ε 3 = ε zz =
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More information2. Mechanics of Materials: Strain. 3. Hookes's Law
Mechanics of Materials Course: WB3413, Dredging Processes 1 Fundamental Theory Required for Sand, Clay and Rock Cutting 1. Mechanics of Materials: Stress 1. Introduction 2. Plane Stress and Coordinate
More informationMECH 5312 Solid Mechanics II. Dr. Calvin M. Stewart Department of Mechanical Engineering The University of Texas at El Paso
MECH 5312 Solid Mechanics II Dr. Calvin M. Stewart Department of Mechanical Engineering The University of Texas at El Paso Table of Contents Thermodynamics Derivation Hooke s Law: Anisotropic Elasticity
More informationTopics. GG612 Structural Geology Sec3on Steve Martel POST 805 Lecture 4 Mechanics: Stress and Elas3city Theory
GG612 Structural Geology Sec3on Steve Martel POST 805 smartel@hawaii.edu Lecture 4 Mechanics: Stress and Elas3city Theory 11/6/15 GG611 1 Topics 1. Stress vectors (trac3ons) 2. Stress at a point 3. Cauchy
More informationModule 5: Laminate Theory Lecture 17: Laminate Constitutive Relations. The Lecture Contains: Laminate Constitutive Relations
Lecture 17: Laminate Constitutive Relations The Lecture Contains: Laminate Constitutive Relations Classification of Laminates CrossPly Laminates Specially Orthotropic Laminates Examples Homework References
More informationStress transformation and Mohr s circle for stresses
Stress transformation and Mohr s circle for stresses 1.1 General State of stress Consider a certain body, subjected to external force. The force F is acting on the surface over an area da of the surface.
More informationME 243. Lecture 10: Combined stresses
ME 243 Mechanics of Solids Lecture 10: Combined stresses Ahmad Shahedi Shakil Lecturer, Dept. of Mechanical Engg, BUET Email: sshakil@me.buet.ac.bd, shakil6791@gmail.com Website: teacher.buet.ac.bd/sshakil
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationMechanics of Earthquakes and Faulting
Mechanics of Earthquakes and Faulting www.geosc.psu.edu/courses/geosc508 Overview Milestones in continuum mechanics Concepts of modulus and stiffness. Stressstrain relations Elasticity Surface and body
More informationELASTICITY (MDM 10203)
LASTICITY (MDM 10203) Lecture Module 5: 3D Constitutive Relations Dr. Waluyo Adi Siswanto University Tun Hussein Onn Malaysia Generalised Hooke's Law In one dimensional system: = (basic Hooke's law) Considering
More informationContinuum mechanism: Stress and strain
Continuum mechanics deals with the relation between forces (stress, σ) and deformation (strain, ε), or deformation rate (strain rate, ε). Solid materials, rigid, usually deform elastically, that is the
More informationStrain Transformation equations
Strain Transformation equations R. Chandramouli Associate DeanResearch SASTRA University, Thanjavur613 401 Joint Initiative of IITs and IISc Funded by MHRD Page 1 of 8 Table of Contents 1. Stress transformation
More information2.2 Relation Between Mathematical & Engineering Constants Isotropic Materials Orthotropic Materials
Chapter : lastic Constitutive quations of a Laminate.0 Introduction quations of Motion Symmetric of Stresses Tensorial and ngineering Strains Symmetry of Constitutive quations. ThreeDimensional Constitutive
More informationGetting Started with Composites Modeling and Analysis
Getting Started with Composites Modeling and Analysis IN THIS WEBINAR: PRESENTED BY: Orthotropic materials and how to define them Composite Laminate properties and modeling Composite failure theories and
More informationIntroduction, Basic Mechanics 2
Computational Biomechanics 18 Lecture : Introduction, Basic Mechanics Ulli Simon, Lucas Engelhardt, Martin Pietsch Scientific Computing Centre Ulm, UZWR Ulm University Contents Mechanical Basics Moment
More informationGG611 Structural Geology Sec1on Steve Martel POST 805
GG611 Structural Geology Sec1on Steve Martel POST 805 smartel@hawaii.edu Lecture 5 Mechanics Stress, Strain, and Rheology 11/6/16 GG611 1 Stresses Control How Rock Fractures hkp://hvo.wr.usgs.gov/kilauea/update/images.html
More informationCHAPTER 4 Stress Transformation
CHAPTER 4 Stress Transformation ANALYSIS OF STRESS For this topic, the stresses to be considered are not on the perpendicular and parallel planes only but also on other inclined planes. A P a a b b P z
More information19. Principal Stresses
19. Principal Stresses I Main Topics A Cauchy s formula B Principal stresses (eigenvectors and eigenvalues) C Example 10/24/18 GG303 1 19. Principal Stresses hkp://hvo.wr.usgs.gov/kilauea/update/images.html
More informationProf. B V S Viswanadham, Department of Civil Engineering, IIT Bombay
50 Module 4: Lecture 1 on Stressstrain relationship and Shear strength of soils Contents Stress state, Mohr s circle analysis and Pole, Principal stressspace, Stress pathsin pq space; MohrCoulomb failure
More informationVYSOKÁ ŠKOLA BÁŇSKÁ TECHNICKÁ UNIVERZITA OSTRAVA
VYSOKÁ ŠKOLA BÁŇSKÁ TECHNICKÁ UNIVERZITA OSTRAVA FAKULTA METALURGIE A MATERIÁLOVÉHO INŽENÝRSTVÍ APPLIED MECHANICS Study Support Leo Václavek Ostrava 2015 Title:Applied Mechanics Code: Author: doc. Ing.
More informationSEMM Mechanics PhD Preliminary Exam Spring Consider a twodimensional rigid motion, whose displacement field is given by
SEMM Mechanics PhD Preliminary Exam Spring 2014 1. Consider a twodimensional rigid motion, whose displacement field is given by u(x) = [cos(β)x 1 + sin(β)x 2 X 1 ]e 1 + [ sin(β)x 1 + cos(β)x 2 X 2 ]e
More informationSound Propagation through Media. Nachiketa Tiwari Indian Institute of Technology Kanpur
Sound Propagation through Media Nachiketa Tiwari Indian Institute of Technology Kanpur LECTURE13 WAVE PROPAGATION IN SOLIDS Longitudinal Vibrations In Thin Plates Unlike 3D solids, thin plates have surfaces
More informationProf. B V S Viswanadham, Department of Civil Engineering, IIT Bombay
51 Module 4: Lecture 2 on Stressstrain relationship and Shear strength of soils Contents Stress state, Mohr s circle analysis and Pole, Principal stressspace, Stress pathsin pq space; Mohrcoulomb failure
More informationConstitutive Equations
Constitutive quations David Roylance Department of Materials Science and ngineering Massachusetts Institute of Technology Cambridge, MA 0239 October 4, 2000 Introduction The modules on kinematics (Module
More informationFracture Mechanics, Damage and Fatigue: Composites
University of Liège Aerospace & Mechanical Engineering Fracture Mechanics, Damage and Fatigue: Composites Ludovic Noels Computational & Multiscale Mechanics of Materials CM3 http://www.ltascm3.ulg.ac.be/
More information8 Properties of Lamina
8 Properties of Lamina 8 ORTHOTROPIC LAMINA An orthotropic lamina is a sheet with unique and predictable properties and consists of an assemblage of fibers ling in the plane of the sheet and held in place
More informationTensor Visualization. CSC 7443: Scientific Information Visualization
Tensor Visualization Tensor data A tensor is a multivariate quantity Scalar is a tensor of rank zero s = s(x,y,z) Vector is a tensor of rank one v = (v x,v y,v z ) For a symmetric tensor of rank 2, its
More informationComparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost
Comparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost 1 Mihir A. Mehta, 2 Satyen D. Ramani 1 PG Student, Department
More informationLaminated Beams of Isotropic or Orthotropic Materials Subjected to Temperature Change
United States Department of Agriculture Forest Service Forest Products Laboratory Research Paper FPL 375 June 1980 Laminated Beams of Isotropic or Orthotropic Materials Subjected to Temperature Change
More information6. Bending CHAPTER OBJECTIVES
CHAPTER OBJECTIVES Determine stress in members caused by bending Discuss how to establish shear and moment diagrams for a beam or shaft Determine largest shear and moment in a member, and specify where
More informationMECH 5312 Solid Mechanics II. Dr. Calvin M. Stewart Department of Mechanical Engineering The University of Texas at El Paso
MECH 5312 Solid Mechanics II Dr. Calvin M. Stewart Department of Mechanical Engineering The University of Texas at El Paso Table of Contents Preliminary Math Concept of Stress Stress Components Equilibrium
More informationBone Tissue Mechanics
Bone Tissue Mechanics João Folgado Paulo R. Fernandes Instituto Superior Técnico, 2016 PART 1 and 2 Introduction The objective of this course is to study basic concepts on hard tissue mechanics. Hard tissue
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationTHERMAL STRESS ANALYSIS OF A FIBEREPOXY COMPOSITE MATERIAL
HERMAL SCIENCE, Year 2011, Vol. 15, No. 2, pp. 559563 559 HERMAL SRESS ANALYSIS OF A FIBEREPOXY COMPOSIE MAERIAL by Radoljub P. OMI] a, Aleksandar S. SEDMAK b*, Dobrivoje M. ]AI] c, Marko V. MILOŠ b,
More informationJeff Brown Hope College, Department of Engineering, 27 Graves Pl., Holland, Michigan, USA UNESCO EOLSS
MECHANICS OF MATERIALS Jeff Brown Hope College, Department of Engineering, 27 Graves Pl., Holland, Michigan, USA Keywords: Solid mechanics, stress, strain, yield strength Contents 1. Introduction 2. Stress
More informationModule #3. Transformation of stresses in 3D READING LIST. DIETER: Ch. 2, pp Ch. 3 in Roesler Ch. 2 in McClintock and Argon Ch.
HOMEWORK From Dieter 3, 4, 37 Module #3 Transformation of stresses in 3D READING LIST DIETER: Ch., pp. 736 Ch. 3 in Roesler Ch. in McClintock and Argon Ch. 7 in Edelglass The Stress Tensor z z x O
More informationUnit 13 Review of Simple Beam Theory
MIT  16.0 Fall, 00 Unit 13 Review of Simple Beam Theory Readings: Review Unified Engineering notes on Beam Theory BMP 3.8, 3.9, 3.10 T & G 1015 Paul A. Lagace, Ph.D. Professor of Aeronautics & Astronautics
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationComb resonator design (2)
Lecture 6: Comb resonator design () Intro Intro. to Mechanics of Materials School of Electrical l Engineering i and Computer Science, Seoul National University Nano/Micro Systems & Controls Laboratory
More informationAnalysis of NonRectangular Laminated Anisotropic Plates by Chebyshev Collocation Method
146 Analysis of NonRectangular Laminated Anisotropic Plates by Chebyshev Collocation Method ChihHsun LIN and MingHwa R. JEN The purpose of this work is to solve the governing differential equations
More informationGG612 Lecture 3. Outline
GG61 Lecture 3 Strain and Stress Should complete infinitesimal strain by adding rota>on. Outline Matrix Opera+ons Strain 1 General concepts Homogeneous strain 3 Matrix representa>ons 4 Squares of line
More informationA DARK GREY P O N T, with a Switch Tail, and a small Star on the Forehead. Any
Y Y Y X X «/ YY Y Y ««Y x ) & \ & & } # Y \#$& / Y Y X» \\ / X X X x & Y Y X «q «z \x» = q Y # % \ & [ & Z \ & { + % ) / / «q zy» / & / / / & x x X / % % ) Y x X Y $ Z % Y Y x x } / % «] «] # z» & Y X»
More informationMECHANICS OF MATERIALS
00 The McGrawHill Companies, Inc. All rights reserved. T Edition CHAPTER MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Teas Tech Universit
More informationNDT&E Methods: UT. VJ Technologies CAVITY INSPECTION. Nondestructive Testing & Evaluation TPU Lecture Course 2015/16.
CAVITY INSPECTION NDT&E Methods: UT VJ Technologies NDT&E Methods: UT 6. NDT&E: Introduction to Methods 6.1. Ultrasonic Testing: Basics of ElastoDynamics 6.2. Principles of Measurement 6.3. The PulseEcho
More informationChapter 3. Load and Stress Analysis
Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3
More informationMECHANICS OF COMPOSITE STRUCTURES
MECHANICS OF COMPOSITE STRUCTURES LÁSZLÓ P. KOLLÁR Budapest University of Technology and Economics GEORGE S. SPRINGER Stanford University PUBLISHED BY THE PRESS SYNDICATE OF THE UNIVERSITY OF CAMBRIDGE
More informationEFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES
EFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES OF WOOD OR PLYWOOD CONSIDERED AS ORTHOTROPIC MATERIALS Information Revied and Reaffirmed March 1956 No. 1510 EFFECT OF ELLIPTIC
More informationEffect of Thermal Stresses on the Failure Criteria of Fiber Composites
Effect of Thermal Stresses on the Failure Criteria of Fiber Composites Martin Leong * Institute of Mechanical Engineering Aalborg University, Aalborg, Denmark Bhavani V. Sankar Department of Mechanical
More information7.3 Design of members subjected to combined forces
7.3 Design of members subjected to combined forces 7.3.1 General In the previous chapters of Draft IS: 800 LSM version, we have stipulated the codal provisions for determining the stress distribution in
More informationMechanical Properties of Materials
Mechanical Properties of Materials Strains Material Model Stresses Learning objectives Understand the qualitative and quantitative description of mechanical properties of materials. Learn the logic of
More information1 Stress and Strain. Introduction
1 Stress and Strain Introduction This book is concerned with the mechanical behavior of materials. The term mechanical behavior refers to the response of materials to forces. Under load, a material may
More informationMAE 323: Lecture 1. Review
This review is divided into two parts. The first part is a minireview of statics and solid mechanics. The second part is a review of matrix/vector fundamentals. The first part is given as an refresher
More informationLAMINATE DESIGN WITH NONSTANDARD PLY ANGLES FOR OPTIMISED INPLANE PERFORMANCE
21 st International Conference on Composite Materials Xi an, 2025 th August 2017 LAMINATE DESIGN WITH NONSTANDARD PLY ANGLES FOR OPTIMISED INPLANE PERFORMANCE Mark W.D. Nielsen 1, Kevin J. Johnson 1,
More informationRock Rheology GEOL 5700 Physics and Chemistry of the Solid Earth
Rock Rheology GEOL 5700 Physics and Chemistry of the Solid Earth References: Turcotte and Schubert, Geodynamics, Sections 2.1,2.4, 2.7, 3.13.8, 6.1, 6.2, 6.8, 7.17.4. Jaeger and Cook, Fundamentals of
More informationDYNAMIC FAILURE ANALYSIS OF LAMINATED COMPOSITE PLATES
Association of Metallurgical Engineers of Serbia AMES Scientific paper UDC:669.1419:628.183=20 DYNAMIC FAILURE ANALYSIS OF LAMINATED COMPOSITE PLATES J. ESKANDARI JAM 1 and N. GARSHASBI NIA 2 1 Aerospace
More informationTHE NETTING ANALYSIS AS A LIMIT CASE OF THE LAMINATED STRUCTURE THEORY
THE NETTING ANALYSIS AS A LIMIT CASE OF THE LAMINATED STRUCTURE THEORY G. Verchery Pluralis, SaintÉtienne, France Georges.Verchery@m4x.org Keywords: netting analysis, classical laminated plate theory,
More informationCONSTITUTIVE RELATIONS FOR LINEAR ELASTIC SOLIDS
Chapter 9 CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS Figure 9.1: Hooke memorial window, St. Helen s, Bishopsgate, City of London 211 212 CHAPTR 9. CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS 9.1 Mechanical
More informationModule 3: 3D Constitutive Equations Lecture 10: Constitutive Relations: Generally Anisotropy to Orthotropy. The Lecture Contains: Stress Symmetry
The Lecture Contains: Stress Symmetry Strain Symmetry Strain Energy Density Function Material Symmetry Symmetry with respect to a Plane Symmetry with respect to two Orthogonal Planes Homework References
More informationGG303 Lecture 6 8/27/09 1 SCALARS, VECTORS, AND TENSORS
GG303 Lecture 6 8/27/09 1 SCALARS, VECTORS, AND TENSORS I Main Topics A Why deal with tensors? B Order of scalars, vectors, and tensors C Linear transformation of scalars and vectors (and tensors) II Why
More informationFlexuralTorsional Buckling of General ColdFormed Steel Columns with Unequal Unbraced Lengths
Proceedings of the Annual Stability Conference Structural Stability Research Council San Antonio, Texas, March 2124, 2017 FlexuralTorsional Buckling of General ColdFormed Steel Columns with Unequal
More informationPEAT SEISMOLOGY Lecture 2: Continuum mechanics
PEAT8002  SEISMOLOGY Lecture 2: Continuum mechanics Nick Rawlinson Research School of Earth Sciences Australian National University Strain Strain is the formal description of the change in shape of a
More informationFree Vibration Response of a Multilayer Smart Hybrid Composite Plate with Embedded SMA Wires
11(2014) 279298 Free Vibration Response of a Multilayer Smart Hybrid Composite Plate with Embedded SMA Wires Abstract In this paper, free vibration response of a hybrid composite plate was studied. Effects
More informationHIGHERORDER THEORIES
HIGHERORDER THEORIES THIRDORDER SHEAR DEFORMATION PLATE THEORY LAYERWISE LAMINATE THEORY J.N. Reddy 1 ThirdOrder Shear Deformation Plate Theory Assumed Displacement Field µ u(x y z t) u 0 (x y t) +
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationEquilibrium of Deformable Body
Equilibrium of Deformable Body Review Static Equilibrium If a body is in static equilibrium under the action applied external forces, the Newton s Second Law provides us six scalar equations of equilibrium
More informationIntroduction to Seismology Spring 2008
MIT OpenCourseWare http://ocw.mit.edu 12.510 Introduction to Seismology Spring 2008 For information about citing these materials or our Terms of Use, visit: http://ocw.mit.edu/terms. Stress and Strain
More informationPressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials
Pressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials Pressure Vessels: In the previous lectures we have discussed elements subjected
More informationComb Resonator Design (2)
Lecture 6: Comb Resonator Design () Intro. to Mechanics of Materials Sh School of felectrical ti lengineering i and dcomputer Science, Si Seoul National University Nano/Micro Systems & Controls Laboratory
More information